| ||Format||Pages||Price|| |
|8||$45.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$45.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$54.00||  ADD TO CART|
Significance and Use
4.1 Carbon black morphology significantly affects the transient and end-use properties of carbon black loaded polymer systems. A carbon black’s particle size distribution is its single most important property, and it relates to degree of blackness, rubber reinforcement, and ability to impart UV protection. For a given loading of carbon black, blackness, reinforcement, and UV protection increase with smaller particle size. Aggregate size and shape (structure) also affect a carbon black's end-use performance, as higher carbon black structure increases viscosity and improves dispersion. The stiffness (modulus) of elastomer systems becomes significantly higher with increasing structure. The preferred method for measuring carbon black morphology (for example, size and shape) is transmission electron microscopy (TEM), but due to the semi-quantitative nature of TEM, it is not suited for mean particle size (MPS) certification. While useful morphological information can be obtained from TEM measurements within a laboratory, due to their inherent between-laboratory variability, TEM generated values should not be used for specification purposes.
4.2 Certification of carbon blacks for UV protection (weatherability) in certain plastics applications has historically been performed using TEM generated mean particle size values. ASTM Committee D24 has demonstrated that due to challenges with obtaining quantitative primary particle size data, particularly between laboratories, a qualification test based on surface area has been implemented, as detailed in Test Method B.
4.3 Carbon black aggregate dimensional and shape properties are dependent upon the nature of the system in which the sample is dispersed, as well as the mixing procedure.
1.1 This test method covers (1) the morphological (for example, size and shape) characterization of carbon black from transmission electron microscope images which are used to derive the mean particle and aggregate size of carbon black in the dry (as manufactured) state, from CAB chip dispersion or removed from a rubber compound and (2) the certification of mean particle size using a correlation based on statistical thickness surface area measurements.
1.2 The values stated in SI units are to be regarded as the standard. The values in parentheses are for information only.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D3349 Test Method for Absorption Coefficient of Ethylene Polymer Material Pigmented with Carbon Black
D6556 Test Method for Carbon Black--Total and External Surface Area by Nitrogen Adsorption
ICS Number Code 83.040.20 (Rubber compounding ingredients)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D3849-14a, Standard Test Method for Carbon Black—Morphological Characterization of Carbon Black Using Electron Microscopy, ASTM International, West Conshohocken, PA, 2014, www.astm.orgBack to Top